The Crystal-Chemical Features of Phases and the Nature of the Coordination Bond in the System [CuxNi(1 x){N(CH2PO3)3}]Na4 nH2O (x = 01)
Somov, N.V.; Chausov, F.F.; Lomova, N.V.; Vorobyov, V.L.; Kazantseva, I.S.; Sapozhnikov, G.V.; Zakirova, R.M.; CRYSTALLOGRAPHY REPORTS 65 (2020) 726–739; doi:10.1134/S1063774520050211

data_1564835
_publ_section_title
;
 The Crystal-Chemical Features of Phases and the Nature of the
 Coordination Bond in the System [CuxNi(1 x){N(CH2PO3)3}]Na4 nH2O (x = 01)
;
_journal_issue                   5
_journal_name_full
;
 CRYSTALLOGRAPHY REPORTS
;
_journal_page_first              726
_journal_page_last               739
_journal_paper_doi               10.1134/S1063774520050211
_journal_volume                  65
_journal_year                    2020
_chemical_formula_sum            'C3 H32 Cu0.23 N Na4 Ni0.77 O22 P3'
_chemical_formula_weight         678.97
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   difmap
_audit_creation_date             2018-09-10T11:58:34-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_cell_angle_alpha                84.785(2)
_cell_angle_beta                 79.504(2)
_cell_angle_gamma                66.971(2)
_cell_formula_units_Z            2
_cell_length_a                   10.0118(2)
_cell_length_b                   11.0311(3)
_cell_length_c                   12.3038(3)
_cell_measurement_reflns_used    17859
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      32.43
_cell_measurement_theta_min      2.633
_cell_volume                     1229.34(5)
_computing_cell_refinement       'CrysAlisPro 1.171.39.8e (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.39.8e (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.39.8e (Rigaku OD, 2015)'
_computing_structure_refinement  'SHELXL-2018/1 (Sheldrick, 2018)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      100(2)
_diffrn_detector                 'CCD plate'
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB Pro: Kappa single'
_diffrn_measurement_method       '\w scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.0599022
_diffrn_orient_matrix_UB_12      -0.0296073
_diffrn_orient_matrix_UB_13      -0.0424804
_diffrn_orient_matrix_UB_21      0.0317208
_diffrn_orient_matrix_UB_22      -0.0526145
_diffrn_orient_matrix_UB_23      0.0367973
_diffrn_orient_matrix_UB_31      -0.038565
_diffrn_orient_matrix_UB_32      -0.0351979
_diffrn_orient_matrix_UB_33      -0.0167468
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0514
_diffrn_reflns_av_unetI/netI     0.0737
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            38565
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.507
_diffrn_reflns_theta_min         2.648
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    1.17
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.57542
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
        CrysAlisPro 1.171.39.8e (Rigaku Oxford Diffraction, 2015)
        Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.834
_exptl_crystal_description       prism
_exptl_crystal_F_000             700
_exptl_crystal_size_max          0.143
_exptl_crystal_size_mid          0.124
_exptl_crystal_size_min          0.066
_refine_diff_density_max         0.598
_refine_diff_density_min         -0.386
_refine_diff_density_rms         0.071
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.013
_refine_ls_hydrogen_treatment    refall
_refine_ls_matrix_type           full
_refine_ls_number_parameters     448
_refine_ls_number_reflns         7512
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.013
_refine_ls_R_factor_all          0.0315
_refine_ls_R_factor_gt           0.025
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0268P)^2^+0.2203P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0584
_refine_ls_wR_factor_ref         0.0606
_reflns_Friedel_coverage         0
_reflns_number_gt                6583
_reflns_number_total             7512
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            tmp611jqdbe
_cod_data_source_block           ni3_4cu1_4atmp_2
_cod_database_code               1564835